JOURNAL OF FOREST SCIENCE, 62, 2016 (11): 521–528
Beech sawn timber for structural use: A case study
for mechanical characterization and optimization
of the Italian visual strength grading rule
D. Cibecchini, A. Cavalli, G. Goli, M. Togni
Department of Agricultural, Food and Forestry Systems (GESAAF), School of Agriculture, University of Florence, Florence, Italy
ABSTRACT: The potential use of beech (Fagus sylvatica Linnaeus) sawn timber for structures has been investigated. Beech stands in transition from coppice to high forest after thinning interventions have been sampled from different Italian sources. A sample of 160 beams of two different cross sections was extracted and tested, according to the nor-malized procedures for the characterization of wood for structures. The specimens were visually graded considering the strength relevant defects, according to the Italian standard. To determine the mechanical properties of the timber (namely strength and stiffness), four-point bending tests were performed and the main characteristic values were derived. The results of the study reveal that knot ratio was the principal defect that influenced both resistance and yields. The potential strength class D30 was achieved with the resulting characteristic values, although, due to the small number of samples tested, the reached class could not be formally assigned. To improve the effectiveness of the grading rule in the Italian standard, some modifications and a new grade were proposed for the beech sawn timber. Finally the D40 strength class could be theoretically reached, but with reduced yields.
Keywords: Fagus sylvatica; grade; modulus of elasticity; modulus of rupture; strength class; strength determining defect
The beech (Fagus sylvatica Linnaeus) wood has not yet been used for structural purposes in Italy, even though it is widespread in Italy and in Europe, and offers outstanding technological properties (Lo Monaco et al. 2014) and many non-structural applications. On the contrary, this hardwood pro-vokes a strong interest in Europe where it is already utilized for load-bearing structures (Aicher et al. 2013). Therefore, several studies have focused on its mechanical performances as solid sawn tim-ber (Frühwald, Schickhofer 2004; Frühwald 2008; Lagaňa, Rohanová 2011; Lagaňa, Ba-biak 2012; Widmann et al. 2012), glued laminat-ed timber (Frühwald et al. 2003; Frese, Blass 2005; Ohnesorge et al. 2009; Aicher, Ohne- sorge 2010) and laminated veneer lumber (Knorz, van de Kuilen 2012). The standard EN 1912:2012 about visual strength graded timbers in-cludes the German beech. Moreover, the German Institute of Civil Engineering in Berlin has issued the technical building approvals Z-9.1-679 for glulam of beech timber, and Z-9.1-837 for beech
laminated veneer lumber. However, due to its low natural durability and high shrinkage/swelling co-efficients, the glue laminated timber can currently be used only in service class 1, according to Euro-code 5 (EN 1995-1-1:2004).
The aims of this work are: (i) the assessment of the potential of Italian beech lumber for structural purposes through physical and mechanical charac-terization, (ii) the assessment of the ability of the current Italian visual strength grading standard in classifying the beech wood and finally, where ap-propriate, (iii) to propose improvements of the spe-cific rule, suitable for beech structural beams.
MATERIAL AND METHODS
density with repeated thinning of the shoots. Data about the stands are reported in Table 1.
19 trees were harvested for the research, 10 from Tuscany and 9 from Liguria. They were selected simulating a new thinning operation. From each trunk only the first log was used and delivered to the sawmill. Logs were sawn using a plain-sawn cutting pattern to achieve large planks that for dimensions could be used in joinery. From the planks were ob-tained 160 beams 2.5 m long, with two different cross sections (Table 2). Timber was air seasoned for two years. The surfaces of the beams were not planed.
Visual grading and mechanical testing. The
sam-ples were graded by the rule “Hardwood” of the Ital-ian grading standard UNI 11035-2:2010, considering only the strength determining characteristics: knots, slope of grain, density and shrinkage fissures going through the thickness. Regarding the slope of grain, more in detail, the general grain angle was measured by a scribing test or shrinkage cracks, if present, on a length of 1 m, according to the standard. Because of the variable slope of the grain, likely due to the agamic origin of the forest where the specimens were sampled, it was difficult to measure correctly a gen-eral grain inclination. Thus, in the course of mechan-ical tests, for the beams failed because of the slope of grain, the grain deviation was measured again following the fracture pattern (the worst inclination was assessed) in order to compare it with that one detected during the visual strength grading. The two criteria considering wanes and deformations, given in the rule, were excluded from this grading pattern because many studies proved that they do not have any effect on the mechanical properties (Bonamini, Togni 1999; Ranta-Maunus 1999; Brunetti et al. 2013; Togni et al. 2013) although they could have some negative outcomes during the assembling on a building site. Decay and insect attacks were rejected by the visual grading because not acceptable. Since the relationship between density and annual ring
width in beech is not expected to be inverse (e.g. Bouriaud et al. 2004), the actual rule disregards the measurements of the ring width because this param-eter is overcome by the direct density dparam-etermination. The principal mechanical properties of the speci-mens, namely local modulus of elasticity in bending (modulus of elasticity – MOE) and bending strength (modulus of rupture – MOR), were determined ac-cording to the European standard EN 408:2010. The tests were carried out by means of a universal testing machine (METRO COM Engineering s.p.a., Gar-bagna Novarese, Italy; 200 kN), using some linear variable displacement transducers (Monitran Ltd., Penn, United Kingdom) for measuring the defor-mations under loading conditions. For each sample, two small clear woods were cut as close as possible to the point of rupture for the physical character-ization. In addition, the strength determining defect and the failure mode were recorded. The density and the moisture content of specimens were determined as indicated by the standards ISO 3131:1985 and EN 13183-1:2003, respectively. Edgewise bending tests were performed on the beams graded as S (struc-tural) in accordance with the Italian grading rule “Hardwood”. The characteristic values of the bend-ing strength, modulus of elasticity and density were calculated for the beams selected in the S grade, ac-cording to the European guideline EN 384:2010. The factor for adjusting the characteristic value of the MOR to the size of the sample and to the number of samples (ks) was not applied. This choice was justi-fied by the necessity to check the feasibility of this species for structural uses, considering this test only as the first attempt needed to set a program on fu-ture tests and a suitable extended sampling. For these reasons, the strength classes successively assigned have to be considered as provisional allocations.
RESULTS AND DISCUSSION Visual grading
The graphical and numerical results of visual strength grading are presented in Fig. 1. They show that the structural quality of the Tuscan sample was better than that of the Ligurian sample: 76 and 54% of specimens were assigned to the S grade, respec-Table 2. Cross section and size of the sampled beams
Region Cross section Total
85 × 55 mm 120 × 55 mm
Tuscany 42 50 92
Liguria 43 25 68
Total 85 75 160
Table 1. Main characteristics of forest stands
Region (m a.s.l.)Altitude Fertility coppice cut) (yr)Age (last stock (m³)Growing thinning(s) (yr)Age of Thinning intensity
Tuscany 1,150–1,350 medium 75 485 37–66 moderate
tively. Among the considered characteristics, only the size of knots, which is connected with the stand history (coppices in origin) and the silvicultural practices, caused the rejection of the beams. The worst strength quality was found for the specimens of 85 × 55 mm nominal cross section that repre-sented 54 and 69% of the total beams discarded from the Tuscan and the Ligurian sample,
respec-tively. From the whole sample only two-thirds of the beams were accepted for structural uses.
Main mechanical and physical properties
Strength, stiffness and density properties are listed in Table 3. The mean value of the modulus of rupture
Table 3. Summary of the mechanical and physical properties
Tuscany sample Liguria sample
85 × 55 mm 120 × 55 mm whole 85 × 55 mm 120 × 55 mm whole
N 30 40 70 21 16 37
mean 74.1 67.4 70.3 78.4 83.3 80.6
min 24.0 28.0 24.0 34.0 31.3 31.3
max 115 115 115 109 110 110
SD 23.5 18.9 21.1 18.5 18.7 18.4
CV (%) 31.8 28.0 30.0 23.5 22.4 23.0
mean 13.0 13.6 13.3 13.0 13.4 13.1
min 9.07 8.84 8.84 9.65 10.6 9.65
max 15.3 17.2 17.2 15.3 15.9 15.9
SD 1.62 2.30 2.04 14.8 1.52 1.49
CV (%) 12.5 17.0 15.3 11.4 11.4 11.3
mean 691 693 692 747 739 744
min 566 627 566 668 656 656
max 758 805 805 812 810 812
SD 40.7 32.0 35.7 40.0 46.9 42.7
CV (%) 5.89 4.62 5.16 5.36 6.34 5.74
Moisture content (%)
mean 9.95 10.3 10.1 11.0 11.0 10.9
min 9.23 9.49 9.23 9.41 10.4 9.41
max 10.4 10.8 10.8 11.8 11.4 11.8
SD 0.281 0.368 0.371 0.532 0.253 0.432
CV (%) 2.82 3.58 3.66 4.85 2.33 3.96
N – number of specimens, MOR – modulus of rupture, MOE – modulus of elasticity, SD – standard deviation, CV – coefficient of variation, S – structural
Fig. 1. Grading results of the sampled beams (cross section: 85 × 55, 120 × 55 mm; total) according to UNI 11035:2010: Tuscan and Ligurian samples; S – structural grade
Total 85 × 55 mm 120 × 55 mm
Rejected (%) S (%)
0 20 40 60 80 100
S S S
Total 85 × 55 mm 120 × 55 mm
S S S
in Tuscan beams was 70.3 N·mm–2, for the S grade.
For the Ligurian sample, instead, the mean value of the bending strength in the S grade was 80.6 N·mm–2.
The coefficient of variation as well as the range of MOR and MOE of the Ligurian sample were lower in comparison with those of the Tuscan sample. More-over, as illustrated in the box plot graphics (Fig. 2), the specimens with section height 85 mm displayed a higher variability and a more irregular distribution of the MOR values. Finally, the density mean values for both sources were contained in the ranges of variability indicated in literature (Giordano 1981) and the coefficients of variation were low.
The characteristic values of the main mechanical and physical properties were calculated in accor-dance with the procedure given by the European standard EN 384:2010. For each sample, the 5-per-centile non-parametric values (calculated by rank-ing data) of bendrank-ing strength (fm, k) and density (ρk) as well as the mean value of the local modulus of elasticity parallel to grain (E0, mean) were determined.
The 5-percentile of bending strength was adjust-ed to 150 mm depth by the factor kh (EN 384:2010) given in Eq. 1, also to compare it with the other structural timbers collected in the European stan-dard EN 1912:2012:
kh = (150/h)0.2 (1)
h – depth of a bending specimen.
The density and the MOE values were also adjust-ed to 12% moisture content and the local modulus of elasticity was used to calculate the characteristic value of the stiffness – E0, mean (Table 4). Then, all the samples are reconsidered together according to EN 384:2010, with the aim to evaluate the actual potentiality in structure for beech in general. The
synthetic results of the computation of the charac-teristic values are reported in Table 5.
Prospective strength class
In order to evaluate the obtained results, the S grade was informally allocated to a strength class, as listed in EN 338:2016. The resulting characteris-tic values allow reaching the D30 strength class. As described before, this strength class must be consid-ered as a provisional allocation, because of the low number of specimens and because the factor ks was not applied. At present the only structural beech list-ed in EN 1912:2012 is the German one, in the respec-tive strength classes D40 and D35 for grades LS13 and LS10 of the national standard DIN 4074-5:2012. Table 5 also shows the values of the beech selected in the Italian grade in comparison with D30 class.
New visual grading parameters for beech timber
Hence, in order to improve the effectiveness of the Italian standard, an adjustment of the grading rule for the beech timber should be studied. To
Table 4. Characteristic values of graded beech timber – S (structural) grade for each provenance and cross size
Tuscany Liguria Whole sample
120 × 55 mm 85 × 55 mm unique sample 120 × 55 mm 85 × 55 mm
N 40 30 36* 55 51
MOR (fm, 05, N·mm–2) 34.1 24.1 30.2 32.9 28.7
MOE (E0, mean, kN·mm–2) 13.3 12.7 13.0 13.3 12.8
Density (ρ05 , kg·m–3) 637 598 677 646 642
N – number of specimens, MOR – modulus of rupture, fm, 05 – 5-percentile, MOE – modulus of elasticity, E0, mean – mean value of the localmodulus of elasticity parallel to grain, ρ05 – 5-percentile, *one beam was rejected during the mechanical tests due to the failure mode, in bold – values not to be considered for the number of beams lower than 40 (EN 384:2010)
evaluate the main visual characteristics that affect the bending strength, the relations between the mechanical properties and the grading parameters were assessed. Therefore, a correlation matrix was carried out between knot ratio, slope of grain, den-sity and MOR. As shown in Table 6 and in Fig. 3, the best correlation was between MOR and knottiness, concerning the smallest cross section. The ring width, which in theory does not affect density in diffuse-porous hardwoods (Bouriaud et al. 2004), was not considered as a classification criterion for beech timber. No correlation between strength and density was found, as reported also by Frühwald and Schickhofer (2004), Frühwald (2008), and Lagaňa and Rohanová (2011). The resulting cor-relation coefficient for the whole sample between MOR and the values of the slope of grain was not significant. However, excluding the beams where the knot ratio was the reason for failure (51% of the total sample) such a correlation coefficient signifi-cantly increased to R = –0.63 for the whole sample. Frühwald (2008) described the same trend in her research. Hence, as expected, the slope of grain was one of the main strength relevant defects of the tested timber.
Based on these outcomes, a new visual rule for beech was proposed on the basis of the obtained results and a new grade was added for high-lev-el performances called B1 in the standard UNI 11035:2010. The existing grade was renamed B2. For the B1 grade a new knot ratio limit was pro-posed with the threshold 0.25, while the existing one for B2 grade (previously S grade) was left to
the original value 0.5. Consequently, all the other parameters for the each grade have been upgraded. Table 7 shows the grading criteria and the other parameters.
Characteristic values of B1
All the samples were reconsidered together and the data were reprocessed. A new group was formed, taking into account the modified thresh-olds for the B1 grade, with the yield reduced to 42%, and the characteristic values recalculated. With the use of such new grading limits the characteristic value of the sample were enhanced. In fact, the B1 group could be allocated to the D40 strength class, as the characteristic value of the modulus of rup-ture (fm, k) was 46.6 N·mm–2. Conversely, there were
not enough beams included in the B2 grade to cal-culate the characteristic values. The allocation to B1 depended only on the fm, k value (Table 8), because the characteristic values of density (ρk) and stiffness
(E0, mean) were nowise limiting factors to D40.
In order to investigate the potential of the Ital-ian beech timber for load-bearing use and to eval-uate the grading efficiency of the standard UNI 11035:2010, the mechanical characterization of two samples of structural beams, previously visu-ally graded according to the strength properties, Table 5. Characteristic values of the beech timber population – S (structural) grade in comparison with the required value for the D30 strength class
Whole sample Required values for D30 Closeness to D30 values (%)
MOR (fm, k*, N·mm–2) 31.0 30 +3.3
MOE (E0, mean, kN·mm–2) 13.0 11 +18.2
Density (ρk, kg·m–3) 644 530 +21.5
MOR – modulus of rupture, fm, k – characteristic value of bending strength, *factor for adjusting the characteristic value of the MOR to the size of the sample and to the number of samples (ks) not applied, MOE – modulus of elasticity, E0, mean – mean value of the localmodulus of elasticity parallel to grain, ρk – characteristic value of density
Table 6. The values of Pearson’s correlation coefficient for the beech from two regions and for the whole sample
Correlation 120 × 55 mm 85 × 55 mm together 120 × 55 mm 85 × 55 mm togetherTuscany Liguria Whole sample Knot ratio-MOR –0.61*** –0.80*** –0.71*** –0.53*** –0.65*** –0.62*** –0.70***
Slope of grain-MOR ns –0.35** –0.20** –0.50** –0.29** ns ns
Density-MOR ns ns ns ns ns ns ns
was performed. From the obtained results, it can be concluded that:
(i) The mechanical properties of beech full-size sawn timber are very interesting from the aspect of structural uses;
(ii) With the current Italian grading rule, the beams could theoretically be allocated to the D30 strength class;
(iii) Some differences have been found between the sources (37.2% of total rejected beams, 46%
from Liguria and 24% from Tuscany), due to the origin of the stands, in transition from coppice to high forest, and to the management (i.e. the intensity and frequency of thinning). Particular-ly the combined effect involves a high volume of low-quality timber for the irregular shapes of the logs and for the dimension of the knots; (iv) Knots were the visual parameter that mainly
influenced both the mechanical properties and the grading results;
Fig. 3. The scatter plot ma-trix of correlations between strength and visual grading parameters for the whole sample; MOR – modulus of rupture
Table 7. A proposal of the visual strength grading rule for the Italian beech timber
Wane s ≤ 1/3, single knot A ≤ 1/4, d ≤ 40 mm, D ≤ 150 mm, density > 590 kg·m–3, slope of grain ≤ 1/10 (10%). Fissures: shrinkage cracks permitted with restrictions*; ring shakes and cracks due to lightning, frost, lesions not permitted. Fungal decay not permitted. Tension wood no restrictions. Insect damage not permitted. Mistletoe not permitted. Warp: bow 10 mm every 2 m of length; spring 8 mm every 2 m of length; twist 1 mm every 25 mm of width on 2 m of length.
Wane s ≤ 1/3, single knot A ≤ 1/2, d ≤ 70 mm, D ≤ 150 mm, density > 510 kg·m–3, slope of grain ≤ 1/6 (16.5%). Fissures: shrinkage cracks permitted with restrictions*; ring shakes and cracks due to lightning, frost, lesions not permitted. Fungal decay not permitted. Tension wood no restrictions. Insect damage not permitted. Mis-tletoe not permitted. Warp: bow 15 mm every 2 m of length; spring 12 mm every 2 m of length; twist 2 mm every 25 mm of width on 2 m of length.
Table 8. Characteristic values of the beech timber according to the proposed new rule
B1 grade Required values for D40 Closeness to D40 values (%) B2 grade
N 67 39
MOR (fm ,k*, N·mm–2) 46.6 40 +16.5 26.3
MOE (E0, mean, kN·mm–2) 13.6 13 +4.62 12.0
Density (ρk, kg·m–3) 625 550 +13.6 650
N – number of specimens, MOR – modulus of rupture, fm, k – characteristic value of bending strength, *factor for adjusting the characteristic value of the MOR to the size of the sample and to the number of samples (ks) not applied, MOE – modu-lus of elasticity, E0, mean – mean value of the localmodulus of elasticity parallel to grain, ρk – characteristic value of density, D40 – strength class, in bold – values not to be considered for the number of beams lower than 40 (EN 384:2010)
(v) An implementation of the Italian visual grading rule was proposed, adding a new grade for high-level performances of the sawn beams of this species, theoretically reaching the D40 strength class but reducing together the graded sample to 42%.
In conclusion the yields for beams of beech stands seem generally low, because of their ori-gin as coppice, but the structural use can give a valuable contribution to the positive utilization of such kind of forests. The number of tested beams, not large enough to provide definitive results, was adequate for the first assessment of the beech as a structural material. However, in order to actu-ally utilize it, an increase of the number of sam-ples and an extension of the sampling sources are indispensable.
Aicher S., Ohnesorge D. (2010): Shear strength of glued laminated timber made from European beech timber. Eu-ropean Journal of Wood and Wood Products, 69: 143–153. Aicher S., Christian Z., Dill-Langer G. (2013): Hardwood
glulams – emerging timber products of superior mechani-cal properties. In: Salenikovich A. (ed.): Proceedings of World Conference on Timber Engineering, Quebec City, Aug 10–14, 2014: 1–10.
Bonamini G., Togni M. (1999): Classificazione secondo la resistenza e determinazione dei valori caratteristici. In: Il legno di Castagno e di Douglasia della Toscana. Flor-ence, ARSIA: 41–62.
Bouriaud O., Bréda N., Le Moguédec G., Nepveu G. (2004): Modelling variability of wood density in beech as affected by ring age, radial growth and climate. Trees, 18: 264–276. Brunetti M., Nocetti M., Burato P. (2013): Strength proper-ties of chestnut structural timber with wane. Advanced Materials Research, 778: 377–384.
Frese M., Blass H.J. (2005): Beech glulam strength classes. In: Proceeding of 38th Meeting of the International Council
for Research and Innovation in Building and Construc-tion. Working Commission W18 – Timber Structures, Karlsruhe, Aug 28–31, 2005: 1–10.
Frühwald A., Ressel J., Bernasconi A., Becker P., Pitzner B., Wonneman R., Mantau U., Sörgel C., Thoroe C., Dieter M., Englert H. (2003): Hochwertiges Brettschichtholz aus Buchenholz. Hamburg, Bundesforschungsanstalt für Forst- und Holzwirtschaft: 198.
Frühwald K. (2008): Procedure for determination of char-acteristic values of hardwood. Available at http://www. coste53.net/downloads/Oslo/Oslo-WG3/COSTE53-MeetingOslo-WG3-Fruehwald.pdf (accessed July 14, 2016).
Frühwald K., Schickhofer G. (2004): Strength grading of hardwoods. In: Ranta-Maunus A., Toratti T. (eds): Pro-ceedings of the 8th World Conference on Timber Engi-neering, Lahti, June 14–17, 2004: 675–679.
Giordano G. (1981): Tecnologia del legno. Vol. 1. Torino, Unione Tipografico-Editrice Torinese: 853.
Knorz M., van de Kuilen J.W. (2012): Development of a high-capacity engineered wood product – LVL made of European beech (Fagus sylvatica L.). In: Quenneville P. (ed.): Proceeding of the 12th World Conference on Timber Engineering, Auckland, July 15–19, 2012: 487–495. Lagaňa R., Babiak M. (2012): Quality of beech standing trees
related to properties of structural timber. In: Yan I., Liu H. (eds): Proceedings of the 55th International Convention of Society of Wood Science and Technology, Beijing, Aug 27–31, 2012: 1–6.
Lagaňa R., Rohanová A. (2011): Characteristics values of beech timber for potential construction applications. Annals of Warsaw University of Life Sciences – SGGW. Forestry and Wood Technology, 75: 26–29.
Lo Monaco A., Calienno L., Pelosi C., Balletti F., Agresti G., Picchio R. (2014): Technical properties of beech wood from aged coppices in Italy. iForest – Biogeosciences and Forestry, 8: 82–88.
Ranta-Maunus A. (1999): Round Small-diameter Timber for Construction. Espoo, VTT Technical Research Centre of Finland, Ltd.: 210.
Togni M., Cavalli A., Mannozzi D. (2013): Chestnut: From coppice to structural timber. The case study of “Uso Fi-ume” beams sampled in Liguria. Journal of Agricultural Engineering, 44: 1–4.
Widmann R., Fernandez-Cabo J.L., Steiger R. (2012): Me-chanical properties of thermally modified beech timber for structural purposes. European Journal of Wood and Wood Products, 70: 775–784.
Received for publication July 19, 2016 Accepted after corrections September 29, 2016
Prof. Marco Togni, Ph.D., University of Florence, School of Agriculture, Department of Agricultural,